Plasma electrolytic oxidation
Plasma electrolytic oxidation (PEO), also known as microarc oxidation (MAO), is an electrochemical surface treatment process for generating oxide coatings on metals. It is similar to anodizing, but it employs higher potentials, so that discharges occur and the resulting plasma modifies the structure of the oxide layer. This process can be used to grow thick (tens or hundreds of micrometers), largely crystalline, oxide coatings on metals such as aluminium, magnesium and titanium. Because they can present high hardness and a continuous barrier, these coatings can offer protection against wear, corrosion or heat as well as electrical insulation.
The coating is a chemical conversion of the substrate metal into its oxide, and grows both inwards and outwards from the original metal surface. Because it is a conversion coating, rather than a deposited coating (such as a coating formed by plasma spraying), it has excellent adhesion to the substrate metal. A wide range of substrate alloys can be coated, including all wrought aluminium alloys and most cast alloys, although high levels of silicon can reduce coating quality.
Metals such as aluminium naturally form a passivating oxide layer which provides moderate protection against corrosion. The layer is strongly adherent to the metal surface, and it will regrow quickly if scratched off. In conventional anodizing, this layer of oxide is grown on the surface of the metal by the application of electrical potential, while the part is immersed in an acidic electrolyte.
In plasma electrolytic oxidation, higher potentials are applied. For example, in the plasma electrolytic oxidation of aluminium, at least 200 V must be applied. This locally exceeds the dielectric breakdown potential of the growing oxide film, and discharges occur. These discharges result in localised plasma reactions, with conditions of high temperature and pressure which modify the growing oxide. Processes include melting, melt-flow, re-solidification, sintering and densification of the growing oxide. One of the most significant effects, is that the oxide is partially converted from amorphous alumina into crystalline forms such as corundum (α-Al2O3) which is much harder. As a result, mechanical properties such as wear resistance and toughness are enhanced.
The part to be coated is immersed in a bath of electrolyte which usually consists of a dilute alkaline solution such as KOH. It is electrically connected, so as to become one of the electrodes in the electrochemical cell, with the other, being a stainless steel counter-electrode, often the wall of the bath itself.
Potentials of over 200 V are applied between these two electrodes. These may be continuous or pulsed direct current (DC) (in which case the part is simply an anode in DC operation), or alternating pulses (alternating current or "pulsed bi-polar" operation) where the stainless steel counter electrode might just be earthed.
Plasma electrolytic oxide coatings are generally recognized for high hardness, wear resistance, and corrosion resistance. However, the coating properties are highly dependent on the substrate used, as well as on the composition of the electrolyte and the electrical regime used (see 'Equipment used' section, above).
Even on aluminium, the coating properties can vary strongly according to the exact alloy composition. For instance, the hardest coatings can be achieved on 2XXX series aluminium alloys, where the highest proportion of crystalline phase corundum (α-Al2O3) is formed, resulting in hardnesses of ~2000 HV, whereas coatings on the 5XXX series have less of this important constituent and are hence softer. Extensive work is being pursued by Prof. T. W. Clyne at the University of Cambridge to investigate the fundamental electrical and plasma physical processes  involved in this process, having previously elucidated some of the micromechanical (& pore architectural), mechanical and thermal characteristics of PEO coatings.
- ^ a b Dunleavy, C.S.; Golosnoy, I.O.; Curran, J.A.; Clyne, T.W. (2009). "Characterisation of discharge events during plasma electrolytic oxidation". Surface and Coatings Technology 203 (22): 3410. doi:10.1016/j.surfcoat.2009.05.004.
- ^ a b c d Curran, J; Clyne, T (2005). "Thermo-physical properties of plasma electrolytic oxide coatings on aluminium". Surface and Coatings Technology 199 (2–3): 168. doi:10.1016/j.surfcoat.2004.09.037.
- ^ Curran, J.A.; Clyne, T.W. (2006). "Porosity in plasma electrolytic oxide coatings". Acta Materialia 54 (7): 1985. doi:10.1016/j.actamat.2005.12.029.
- ^ Curran, J; Clyne, T (2005). "The thermal conductivity of plasma electrolytic oxide coatings on aluminium and magnesium". Surface and Coatings Technology 199 (2–3): 177. doi:10.1016/j.surfcoat.2004.11.045.
Wikimedia Foundation. 2010.
Look at other dictionaries:
Plasma processing — is a plasma based material processing technology that aims at modifying the chemical and physical properties of a surface.Plasma processing techniques include: *Plasma activation *Plasma modification *Plasma functionalization *Plasma… … Wikipedia
Anodizing — Anodizing, or anodising, is an electrolytic passivation process used to increase the thickness of the natural oxide layer on the surface of metal parts. Anodizing increases corrosion resistance and wear resistance, and provides better adhesion… … Wikipedia
Aluminium oxide — Alumina redirects here. For the company, see Alumina Limited. This article is about aluminium(III) oxide Al2O3. For other uses, see Aluminium oxide (disambiguation). Aluminium oxide … Wikipedia
Coating — is a covering that is applied to the surface of an object, usually referred to as the substrate. In many cases coatings are applied to improve surface properties of the substrate, such as appearance, adhesion, wetability, corrosion resistance,… … Wikipedia
Mao (disambiguation) — Mao Zedong, sometimes called just Mao, was the founder of the People s Republic of China. Mao may also refer to: Mao (surname), Chinese family names Mao (name) Mao (people), one of the scheduled tribes of India Mao (languages), a group of Omotic… … Wikipedia
Surface finishing — is a broad range of industrial processes that alter the surface of a manufactured item to achieve a certain property. Finishing processes may be employed to: improve appearance, adhesion or wettability, solderability, corrosion resistance,… … Wikipedia
List of coating techniques — This list contains an overview of coating techniques for thin film deposition, found in the field of materials science. The techniques can be classified as follows: Chemical vapor deposition (CVD) * Metalorganic vapour phase epitaxy *… … Wikipedia
Substrate (materials science) — Substrate is a term used in materials science to describe the base material on which processing is conducted to produce new film or layers of material such as deposited coatings. A typical substrate might be a metal, onto which a coating might be … Wikipedia
PEO — may refer to: Reckong Peo, the capital of Kinnaur district in India PEO may stand for: Parking enforcement officer Plasma electrolytic oxidation, a surface treatment process for metals Polyethylene oxide, a polymer Old Persian language, per ISO… … Wikipedia
Zinc gluconate — Identifiers CAS number 4468 02 4 … Wikipedia